Effect of Elemental Sulfur on Pitting Corrosion of Steels
Muthukumar Nagu*, Abdullatif Abdulhadi, Abdulrahman Huwaiji and Nayef M Alanazi
Research and Development Center, Saudi Aramco, Dhahran-31311, Saudi Arabia
*Corresponding author: Muthukumar Nagu, Research and Development Center, Saudi Aramco, Dhahran-31311, Saudi Arabia, Tel:
00966138726332; E-mail: firstname.lastname@example.org
Rec date: February 12, 2018; Acc date: March 03, 2018; Pub date: March 12, 2018
Copyright: © 2018 Nagu M, et al. This is an open-access article distributed under the terms of the Creative Commons Attribution License,
which permits unrestricted use, distribution, and reproduction in any medium, provided the original author and source are credited.
Citation: Nagu M, Abdulhadi A, Huwaiji A, Alanazi NM (2018) Effect of Elemental Sulfur on Pitting Corrosion of Steels. Insights Anal Electochem.
This paper focuses on studying the pitting corrosion
tendency of austenitic stainless steels (SS 316 L and NIT
60) and carbon steel (API 5 LX 60) in the presence of
elemental sulfur. The pitting corrosion tendency of alloys
was studied by using cyclic polarization technique at two
different temperatures with and without elemental sulfur.
Surface morphology and corrosion products formed on
the exposed coupons were analyzed by scanning electron
microscopy (SEM) and energy dispersive X-ray (EDX). It
was found that the temperature played major role on
pitting corrosion of alloys in presence of elemental sulfur.
SS 316 L gave high pitting resistance than other tested
alloys (NIT 60 and API 5 LX 60).
Keywords: Elemental sulfur; Pitting corrosion;
Electrochemical method; SEM
Sour gas fields have increasingly been explored and
developed during the last decade due to the increasing energy
demands . Elemental sulfur deposition due to several
chemical and physical facts indicates possibility of dissociation
of hydrogen sulfide or polysulfide to produce elemental sulfur.
Therefore dissociated elemental sulfur start to deposit in the
form of small particles and adheres to the internal surface of
pipelines. Elemental sulfur naturally acts as a cathode to the
steel pipe due to the difference in their potential. An active
electrochemical cell will be established as soon as free water
or conductive condensates pass over the deposited elemental
sulfur particle. When this happens, an accelerated localized
corrosion will take place and initiate a pit [2-4]. The
progression of this pit will be very unlikely to be arrested even
if corrosion inhibitor is injected into the system . Therefore,
a leak of toxic and flammable gases will be expected in such
location. The most common location for elemental sulfur
deposition in natural gas transmission pipelines is immediately
downstream of a point of pressure reduction which is also
associated with temperature reduction . Elemental sulfur
(S8) reacts with water at temperatures of greater than 80°C,
resulting in significant acidification of the corrosion solution
 as shown in Equation 1.
The previous experimental results also showed that steel
was corroded severely when it has a direct contact with wet
elemental sulfur at salt free conditions [7,8]. The most of
researchers reported the gravimetric method to predict the
elemental sulfur corrosion for natural gas pipeline application
. There is a limited publication on electrochemical methods
to predict the pitting tendency of alloy in presence of
The aim of this paper is to use of cyclic polarization
technique to study the pitting corrosion tendency of austenitic
stainless steels (SS 316 L and NIT 60) and carbon steel API 5 LX
60 in presence and absence of elemental sulfur, with particular
emphasis on detection of temperature effects, and
identification of formed corrosion products.
GAMRY Interface 1000 was used for all electrochemical
experiments. The electrochemical cell included a saturated
calomel electrode (SCE) as a reference, a platinum counter
electrode and the test sample as working electrode. The
exposed surface area of the working electrode was 1 cm2.
Open circuit potential and cyclic polarization experiments
(ASTM Standard G 61) were conducted to determine the
pitting tendency of the studied alloys in 3.5% sodium chloride
solution with and without elemental sulfur. To study the
temperature effect at low and high temperatures, 25°C and
80°C were selected in presence of three different steels
namely: SS 316 L, NIT 60 and API 5 LX 60. The chemical
compositions of the studied alloys are listed in Table 1. The
elemental sulfur (about 0.5 gm) was deposited on the polished
Insights in Analytical Electrochemistry
© Copyright iMedPub | This article is available from: http://electroanalytical.imedpub.com/ 1
tested coupons by heating it slightly above its melting-point
(115°C - 120°C) then pouring it onto the coupon surface.
Table 1 Chemical composition of tested alloys.
Alloys Cr Ni Mn Mo Si N C P S Cu
SS 316 L 16-18 14 Max 2 Max 3 Max 0.75 0.01 Max 0.03 0.045 Max 0.03 Max
Nitronic 60 16-18 9 Max 9 Max 0.75 4.00 0.08-0.18 0.10 0.04 0.01 0.75 max
API 5 LX.60 0.3 0.03 0.03
The elemental sulfur deposited working electrode coupon
was assembled in a glass autoclave electrochemical cell. The
test solution (3.5% NaCl) was deaerated using nitrogen gas
during the test period of 7 days and the open circuit potential
was measured for entire test period. Cyclic polarization scan
was then initiated at the end of the incubation period at scan
rate of 0.125 mV/sec.
After the cyclic polarization experiments, Corrosion
potential (Ecorr), Pitting potential (Epit), Repassivation potential
(Erp), overall pitting resistance (ERP), and corrosion current
(Icorr) values were obtained from the cyclic polarization curves.
The tested coupons were removed after terminating the tests
and characterized using scanning electron microscopy (SEM)
and energy dispersive X-ray analysis (EDX). Corrosion products
were then removed by treatment with Clarke solution  and
the localized attack of the tested corrosion coupons were
mapped by 3D DIKTAK surface profilometer. Finally, the overall
pitting resistance value was calculated using the following
Overall pitting resistance(ERP)=Repassivation potential(Erp)-
Results and Discussion
Cyclic polarization measurements were performed in order
to determine the tendency of the tested samples to undergo
localized pitting corrosion with and without elemental sulfur at
25°C and 80°C when placed in 3.5% NaCl solution. The derived
electrochemical data from cyclic polarization experiments
namely; Corrosion potential (Ecorr), Pitting potential (Epit),
Repassivation potential (Erp), overall pitting resistance (ERP),
and corrosion current (Icorr) values of each tested alloys at 80°C
and 25°C, are presented in Tables 2 and 3 respectively.
Table 2 Electrochemical data of various steels in 3.5% NaCl at 80°C.
Alloy Elemental Sulfur (gm) Ecorr(mV) Epit(mV) Erp (mV)
Overall Pitting Resistance ERP=Erp-
SS 316 L 0 -265 111 -256 9 0.02
SS 316 L 0.5 -218 103 -454 -236 0.01
NIT 60 0 -253 -13 -268 -15 0.01
NIT 60 0.5 -581 NA NA NA 20
API 5 LX 60 0 -904 NA NA NA 3.5
API 5 LX 60 0.5 -985 NA NA NA 22
Table 3 Electrochemical data of various steels in 3.5% NaCl solution at 25°C.
Alloy Elemental Sulfur(gm) Ecorr (mV) Epit (mV) Erp (mV)
SS 316 L 0 -300 421 -297 3 0.01
SS 316 L 0.5 -204 338 -400 -196 0.01
NIT 60 0 -222 177 -280 -58 0.02
NIT 60 0.5 -581 39 -365 -222 0.01
API 5 LX 60 0 -869 NA NA NA 0.3
API 5 LX 60 0.5 -726 NA NA NA 400
Insights in Analytical Electrochemistry
ISSN 2470-9867 Vol.4 No.1:6
2 This article is available from: http://electroanalytical.imedpub.com/
Electrochemical behavior of SS 316 L
Figure 1a and 1b show the cyclic polarization curves
obtained in the deaerated 3.5% sodium chloride solution at
25°C and 80°C. Both the tested temperatures, SS 316 L showed
the passive region, where the passive range decreased in
presence of elemental sulfur, indicating that the passive
properties of the films slightly degraded as the temperature
increased. Furthermore, the overall pitting resistance value of
SS 316 L (ERP) at 25°C (Table 3) with sulfur was more negative
(-196 mV) than in the absence of sulfur system (3 mV). It
indicated that SS 316 L was not able to reform the passive film
during the reverse scan (Figure 1b) at 80°C. There was no
much change in the corrosion current (Icorr) values in presence
and absence of sulfur at both 80°C and 25°C.
Figure 1 Cyclic polarization curves of SS 316 L with and
without sulfur at (a) 80°C (b) 25°C in 3.5% NaCl solution.
The morphologies of the pits also showed a significant
change at high temperature in presence of elemental sulfur, as
shown in Figures 2 and 3.
Figure 2 Optical microscope and profilometer images of SS
316 L at 80°C.
Figure 3 Optical microscope and profilometer images of SS
316 L at 25°C.
Stainless steel surfaces are generally rendered passive by
formation of a surface oxides layer. This layer depends on the